### Are Zinc Clusters Really Amorphous? A detailed Protocol for

### Locat-ing Global Minimum Structures of Clusters

### †

### Andr´es Aguado

a,∗### , Andr´es Vega

a### , Alexandre Lebon

b### , and Bernd von Issendorff

cReceived Xth XXXXXXXXXX 20XX, Accepted Xth XXXXXXXXX 20XX

First published on the web Xth XXXXXXXXXX 200X

DOI: 10.1039/b000000x

We report the results of a conjoint experimental/theoretical effort to assess the structures of free-standing zinc clusters with up to
73 atoms. Experiment provides photoemission spectra for Zn−_{N} cluster anions, to be used as fingerprints in structural assessment,
as well as mass spectra for both anion and cation clusters. Theory provides both a detailed description of a novel protocol to locate
global minimum structures of clusters in an efficient and reliable way, and its specific application to neutral and charged zinc
clusters. Our methodology is based on the well-known hybrid EP-DFT (empirical potential-density functional theory) approach,
in which the approximate potential energy surface generated by an empirical Gupta potential is first sampled with unbiased basin
hopping simulations, and then a selection of the isomers so identified is re-optimized at a first-principles DFT level. The novelty
introduced in our paper is a simple but efficient new recipe to obtain the best possible EP parameters for a given cluster system,
with which the first step of the EP-DFT method is to be performed. Our method is able to reproduce experimental measurements
at an excellent level for most cluster sizes, implying its ability to locate the true global minimum structures; meanwhile, if exactly
the same method is applied based on the existing Gupta potential (fitted to bulk properties), it leads to wrong predicted structures
with energies between 1 and 2 eV above the correct ones. Opposite to what was claimed in the past, our work unequivocally
demonstrates that Zn clusters are not amorphous, and they rather adopt high symmetry structures for most sizes. We show that
Zn clusters have a number of exotic, unprecedented structural and electronic properties which are not expected for clusters of a
metallic element, and describe them in detail.

### 1

### Introduction

A key step in predicting and rationalising physico-chemical properties of small clusters and nanoparticles is their structural characterization. This is so because the interesting electronic, magnetic, optical, catalytic, etc., properties of nanoparticles depend on the geometry of the ionic skeleton. To achieve a complete characterization would require an exhaustive sam-pling of the potential energy surface (PES), whose complex-ity (number of local minima) increases in an exponential way with the number of atoms in the nanoparticle. At low temper-ature, the most stable structure is that of the global minimum (GM) on the PES, and most experiments probably involve the GM structure, and maybe a few isomers with low excitation energies. As the structure of a free-standing cluster is not

di-†Electronic Supplementary Information (ESI) available: Atomic coordinates (in xyz format and ˚A units) and point group symmetries for the Global Min-imum structures reported in this paper; full computational details and bench-mark calculations aimed at assessing the accuracy of the level of theory em-ployed. See DOI: 10.1039/b000000x/

a Departamento de F´ısica Te´orica, At´omica y ´Optica, University of Val-ladolid, Valladolid 47071, Spain; E-mail: aguado@metodos.fam.cie.uva.es b Laboratoire Chimie ´Electrochimie Mol´eculaire et Chimie Analytique, UMR CNRS 6521, 29285 Brest Cedex, France

c Physikalisches Institut, Universit¨at Freiburg, H.-Herder-Str. 3, D-79104 Freiburg, Germany

rectly available from experiment, unbiased global optimiza-tion (GO) is essential for the predicoptimiza-tion and later assessment of cluster structures. The structural assessment itself is usually achieved by indirect means, i.e. by comparing the theoretical predictions on several physical observables with experimental measurements (photoemission and vibrational spectra, as well as diffraction patterns and other properties, are considered as good structural “fingerprints”).

local minima on the PES.

Two main types of GO algorithms have been developed. Population-based algorithms deal with a collection of clus-ter structures, and improve the structure of individuals by moving them on the PES according to some rules that try to mimic biological processes in nature. Iteration of those steps evolves the whole population in such a way that only the best fitted individuals (i.e. those with a lower energy) sur-vive, so that if enough iterations are allowed the probability that the best fitted (GM) individual belongs to the popula-tion approaches unity. Evolupopula-tionary algorithms, such as the genetic algorithm1,2and differential evolution3, generate off-springs (new cluster structures) by crossover operations (e.g. “cut-and-splice”) or by mutation of the individuals; the con-vergence rate of these methods is quite sensitive indeed to the specific set of modifications allowed to the individuals. Par-ticle swarm optimization4,5 rather imitates the movement of individuals in a bird flock, and was first intended for simu-lating social behavior. The coordinates and velocities of each individual are updated to approach the currently best individ-ual, and the expectation is that the whole swarm will approach in this way the optimal region of the PES around the GM.

Individual-based GO algorithms start instead the
optimiza-tion from a single cluster and allow that individual to sample
the whole PES in order to identify the GM structure. As
spe-cific examples we mention simulated annealing6, Monte Carlo
minimization, minima hopping7,8, stochastic surface
walk-ing9,10_{and basin hopping (BH)}11–14_{methods. The essence of}
the BH method is a mapping of the original PES into a
step-wise modified surface obtained by local optimization. In the
transformed surface there are plateaus associated with each
lo-cal minimum, and discontinuous steps separating the different
local minima. In this way, energy barriers are substantially
de-creased so that a Monte-Carlo sampling (the second ingredient
in the BH method) is much more efficient than on the original
landscape. Several types of movements can be implemented
to generate new cluster structures and sample the transformed
PES: the basic one is a random change in the atomic
coordi-nates. More specific movements include changes in the
co-ordinates of only surface atoms, or the swap of two different
atomic species in the optimization of the chemical ordering of
nanoalloys, for example. Although in this paper the focus is
on structure optimization using the BH method, we mention
in passing that all these methods can also be employed in
ma-terials design, where one aims to solve the so-called inverse
problem: given a certain desired property, discover (design) a
material that possesses that property under a given set of
con-straints15–18.

Most unbiased GO methods require a huge number of eval-uations of the energy function in order to achieve an efficient (statistically meaningful) sampling of the PES, and for this reason they have been traditionally tested on simple model

surfaces such as those generated by Lennard-Jones, Morse, etc, empirical potentials. But when the goal is to make contact with experimental measurements and deal with realistic sys-tems, sampling an accurate PES becomes indispensable. Then we face an interesting dichotomy and GO methods branch into two different practical implementations. In the first one, the GO method directly samples a quantum accurate description of the PES such as that provided by a density functional the-ory (DFT) method, for example19,20. This allows to have ac-curate energies and forces at all stages of the optimization pro-cess, but greatly increases the cost of exploring the PES com-prehensively. For this reason, the statistical accuracy of the sampling is sacrificed, severely limiting the size of the clus-ters that it is possible to investigate with confidence. In the second implementation, the GO method is initially applied to an approximate PES generated with a low-cost empirical po-tential (EP), which allows a statistically meaningful, extensive search. Then a diversity of the structures located in that search are locally re-optimized at the DFT level to recover accuracy in the PES. In this so-called EP-DFT approach21, the poten-tial danger is that one might be re-optimizing at the DFT level structures that have very low stability on the true PES. If we want to obtain results consistent with experiments, it is imper-ative to train the EP based on first-principles cluster results, a step that is often bypassed simply because there typically are bulk-based parametrizations of the EP available. In this paper, we will show explicitly that transferability of EP parameters is a very serious issue which may lead to unrealistic GM predic-tions in an EP-DFT search, and will propose a simple and sys-tematic method to fit an EP explicitly to DFT results on metal clusters. We will be concerned specifically with the Gupta po-tential22–24 but the results should be generally applicable to other EP’s with a relatively small number of parameters.

The EP-DFT approach can itself be further subdivided into two quite different practical branches: one may decide to use BH or machine learning-like techniques to train a neural-network potential with a huge number of adjustable param-eters in order to ensure high numerical accuracy in the PES generated with the empirical potential25,26. The disadvantage in this method is that the problem becomes a purely numer-ical one and each parameter lacks a precise physnumer-ical mean-ing. We personally prefer to employ an analytic potential with the smallest possible number of parameters compatible with a reasonable level of accuracy in the PES. Even if sacrific-ing some numerical accuracy, the advantage here is that if few parameters generate reasonable physics, then each parameter has a well-defined physical meaning, which allows to identify useful trends and gain physical insight into the properties of metallic nanoparticles. It is for this reason that we decided to employ the Gupta potential, which has just two independent parameters when expressed in reduced units.

clusters. We report putative GM structures for clusters with up to 73 atoms, for both neutral (ZnN) and singly-charged (Zn+N

and Zn−_{N}) clusters, as well as mass and photoemission
spec-tra for cluster anions. One important reason for our choice
is that there are many experimental measurements27–29
(in-cluding previous mass spectra for cations and our own mass
and photoemission spectra for anions) that will serve to
vali-date the theoretical results, and that have not yet been
repro-duced/interpreted by theory. Photoemission spectra provide
very sensitive structural fingerprints, so that a comparison
be-tween DFT results for the electron density of states and the
photoemission spectra is a recognized method for structure
assignment30,31. ZnN clusters are also interesting because in

previous theoretical reports they have been predicted to have
amorphous GM structures32_{, which apparently does not match}
with the well-structured photoemission spectra measured for
anions (a well-structured photoelectron spectrum usually
in-dicates an ordered structure, because degeneracies in the
elec-tron density of states are related with symmetries of the
sys-tem). At a fundamental level, ZnN clusters are also

interest-ing as model systems to analyze the insulator-to-metal tran-sition28: while the Zn2 dimer and small clusters are weakly bound via vdW effects, the bulk is metallic, so an increas-ingsp−hybridization and closing of the HOMO-LUMO gap (the gap between the highest occupied and lowest unnoccu-pied molecular orbitals) is expected as a function of sizeN. At a more applied level, we are initiating studies on Zn-Mg nanoalloys33 because of their excellent corrosion protection properties. The structures of pure Zn clusters are needed as a reference to calculate excess quantities in Zn-Mg nanoalloys in our future research.

### 2

### Experimental and Computational Methods

2.1 Experiment

Zinc cluster anions have been produced in a liquid nitrogen cooled magnetron gas aggregation source, where a pulsed dis-charge at the end of the aggregation tube was used to en-hance the intensity of cluster anions. After exiting the source the clusters were stored in a liquid nitrogen cooled radio fre-quency octupole trap, where the presence of helium buffer gas leads to an efficient cooling of the clusters. After pulsed ex-traction from the trap the cluster ions were size-selected in a double reflection time-of-flight mass spectrometer, decel-erated and irradiated by 6.4 eV photons (or 4.0 eV in some cases) in the interaction region of a magnetic-bottle-type pho-toelectron spectrometer. The spectrometer has been calibrated measuring the known photoelectron spectrum of Pt− ions, which leads to an uncertainty in the measured binding energies of less than 30 meV. A subset of the photoemission spectra has been shown in previous reports27,28,41.

2.2 First-Principles calculations

The main DFT calculations are performed with the SIESTA
code34_{,} _{under the PBE approximation}35 _{to }
exchange-correlation effects. We also employed a van der Waals
cor-rected functional proposed by Klimeˆs et al.36 (KBM
func-tional) in order to check the accuracy of the PBE functional
for selected sizes. We include the 3d semicore states of zinc
in the valence active space and describe the effect of the rest of
core electrons through a norm-conserving pseudopotential
in-cluding non-linear partial core corrections. The cluster
wave-function is expanded into a basis of localized atomic orbitals.
Benchmark accuracy tests demonstrating the high accuracy of
our DFT results, as well as a full description of our
com-putational settings, can be found as Supporting Information
(ESI)†.

Vertical detachment energies (VDE) of the anions are cal-culated through a∆−SCF calculation, that is, as the total en-ergy difference between the anion and the neutral cluster, both clusters adopting the geometry of the anion. In order to sim-ulate the experimental photoelectron spectra, we have broad-ened each line of the KS eigenvalue spectrum by using a Gaus-sian function of width 0.10 eV, which leads to a good agree-ment with experiagree-mental line widths. The calculated electronic density of states (EDOS) was then globally shifted in order to align the binding energy of the highest occupied orbital (the HOMO) with the theoretical VDE value.

2.3 Accurate EP-DFT protocol for global optimization

Putative GM structures are initially determined through unbi-ased BH optimizations11 based on a Gupta empirical poten-tial24. We employ the GMIN code developed by David Wales group37,38. For all cluster sizes, we have performed optimiza-tions in which all atoms are given random displacements at each BH step; for some of the bigger sizes, we have addi-tionally performed “seeded” optimizations in which a high-symmetry core is kept fixed and only the rest of atoms is ac-tive in the optimization. Around 100 competiac-tive structures are then selected for each size and re-optimized at the Kohn-Sham DFT level. The optimizations for neutral, cation and an-ion clusters are completely independent runs. In a final “size-comparison” step, we have always generated new structures for N+1 and N−1 atom clusters by creating a vacancy or adding one adatom to the GM structure of theN−atom clus-ter. This step is directly performed at theab initiolevel. More technical details about the optimization runs can be found in the ESI†.

energies, the results will be useless (or irrelevant when com-pared to experimental results) if the DFT energies are calcu-lated from alocal optimizationof initial structures which sig-nificantly depart from the real ones. For this reason, we have carefully tested the accuracy of the current parameterization of the Gupta potential for zinc24in its application to Zn clusters (we remind the reader that the potential parameters have been fitted only to bulk properties, and transferability is certainly an issue). To simplify the problem, we would like to work with the minimum possible number of relevant parameters, so a first step is simplifying the potential expression as much as possible. The general expression of the Gupta potential energy contains five parameters:

E(ZnN) = N

### ∑

i=1

(E_{i}band+E_{i}rep) (1)

E_{i}band=−

( N

### ∑

j6=i

ξ2exp

−2q(ri j r0

−1)

)1/2

(2)

E_{i}rep=

N

### ∑

j6=i

Aexp

−p(ri j r0

−1)

(3)

whereri jis the distance between atomsiand j. qandp are

dimensionless parameters that determine the effective spatial range of the band and repulsive terms, respectively, whileξ and A fix the strength of those interaction terms and have units of energy. r0 is a scaling factor for the distances be-tween atoms, usually identified with the nearest-neighbor dis-tance in the bulk metal. Although the potential incorporates only isotropic interactions, non-additive (many-body) effects are introduced through the square-root dependence of the at-tractive band energy term on interatomic distances.

L´opez and Jellinek39demonstrated that only four of the five parameters are truly independent in the Gupta potential ex-pression, and so any one of them, for exampler0, can be elim-inated in favor of four new independent parameters. Specifi-cally, we definep0=p/r0,q0=q/r0,A0=Aepandξ0=ξeq. The potential is then rewritten as

Ei= N

### ∑

j6=i

A0exp

−p0ri j− (

N

### ∑

j6=i

ξ02exp−2q0ri j )1/2

. (4)

When considering reduced energy and distance units, only
two independent parameters remain which determine the true
physical content of the Gupta potential40_{.} _{We have }
con-veniently chosen those parameters as λ =q0/p0=q/p and
χ=A0/ξ0= (Aep)/(ξeq). With reduced distances defined as

r∗_{i j}=p0ri j and reduced energies defined asEi∗=
Ei

2ξ0, the re-duced total energy of a cluster is

E∗=1 2 N

### ∑

i N### ∑

j6=i

χexp[r∗_{i j}]−

" N

### ∑

j6=i

exp[−2λr_{i j}∗]

#1/2

. (5)

The two independent parametersλ andχcompletely describe the intrinsic topography of the potential energy landscape, in-cluding the structure and energetic ordering of local minima (isomers). Later on, in the results section, we will show that these parameters have quite well defined physical meanings, and that their physically meaningful ranges of variation are λ ∈(0,0.5)andχ∈(0,∞). Moreover, even ifχ can increase without limit from a mathematical point of view, we have ex-plicitly checked that for each fixed value of λ, there is al-ways a maximum value ofχbeyond which the topography no longer evolves, essentially corresponding to hard-sphere-like systems. Then, in practice,χ∈(0,χmax(λ)].

We have devised a simple but detailed protocol to choose optimal values of the reduced parameters for zinc clusters, but obviously it could be applied to any other homo-atomic metal clusters. It is based on benchmarking the performance of the reduced Gupta potential against DFT results. There might be several ways to implement this idea in practice, and next we describe ours: First, as we are interested in the size range be-low 73 atoms, we choose six evenly distributed but otherwise random sizes in the range N=10−73. DFT calculations aimed to identify the optimal potential will be performed only for those sizes. In second place, and because the parameter space of the reduced Gupta potential is just two-dimensional and bounded, it is a relatively simple and inexpensive mat-ter to perform extensive BH optimizations on a discrete set of (λ,χ)points that provides a representative sample of the whole parameter space. Specifically, we have employed about 100 different potentials withλ values between 0.01 and 0.49, and withχ values between 2 andχmax(λ). For each of those potentials, we have performed structure optimizations on the six chosen cluster sizes. The cost of this part of the protocol might be substantially reduced if one is interested in a specific metal for which there is a Gupta potential already available, typically fitted to bulk properties. Then one might explore just a local environment of(λ,χ)values around that reference point which is appropriate for the bulk. Here we have pre-ferred to explore the whole parameter space in order to keep our approach fully unbiased and not to make any assumptions, but we have founda posteriorithat the optimal parameters for clusters (see below) are not too distant from the bulk-fitted values.

### val-Zn

_{9}

### (D

_{3h}

### )

### Zn

_{10}

### (C

_{3v}

### )

### Zn

_{11}+

### (C

_{3v}

### )

_{Zn}

11

### (D

3h### )

### Zn

11 −### (C

_{s}

### )

### Zn

_{12}+

### (C

_{s}

### )

### Zn

_{12}

### (C

_{s}

### )

_{Zn}

12
−
### (C

_{s}

### )

### Zn

13 +### (C

_{1}

### )

### Zn

_{13}

### (C

_{1}

### )

### Zn

_{13}−

### (C

_{s}

### )

_{Zn}

14
+
### (C

_{s}

### )

### Zn

_{14}

### (C

_{s}

### )

### Zn

_{14}−

### (C

_{1}

### )

### Zn

_{15}+

### (C

_{2}

### −C )

2v### Zn

_{15}

### (C

_{2v}

### )

### Zn

_{16}+

### (C

_{1}

### −C)

s### Zn

_{16}

### (C

_{s}

### )

### Zn

_{16}−

### (C

_{2v}

### )

Fig. 1Putative GM structures and approximate point group symmetries of zinc clusters withN=9−16 atoms. The GM structure of charged

clusters is shown only when it does not coincide with the GM of the corresponding neutral cluster. When the structure of theN−cluster is

obtained by adding one atom to the(N−1)−cluster, the adatom is shown in blue. Blue color is additionally used to highlight that a structure

is obtained by adding several atoms to a common structural motif.

ues ofλ and relatively small values ofχ. Then we have sam-pled, in a second step, a finer grid of(λ,χ)points in that local region. In this way, we have found (see next section) that the best agreement with the DFT results for zinc clusters occurs for a set of optimal reduced parameters which, while being located on the same corner of parameter space as the bulk-fitted parameters, significantly differ from them, implying the bulk parameters are not transferable to clusters. Once the op-timal parameters are located, one can proceed with the usual EP-DFT approach for all sizes. Alternatively, and in order to enhance diversity and so the chances to locate the true GM structure, a good option is to use not only the optimal poten-tial, but a few others in a local environment about the optimal one, to generate candidate structures for DFT re-optimization. Additional technical details about this essential potential opti-mization step are given in the ESI†.

With the new set of parameters, the DFT global minimum is systematically found between the 10-15 most stable Gupta structures for most zinc clusters, which is a very successful re-sult for a potential containing just two parameters. The cluster structures predicted with the bulk parametrization are, on the contrary, between 1 and 2 eV less stable than our putative GM structures when reoptimized at the DFT level, and this is a huge energy error, so the bulk parametrization is simply not representative of the interactions in zinc clusters. This is one of the important new findings reported in this paper, as we

have found that any combined EP/DFT approach based on the bulk Gupta parameters is doomed to fail when applied to the location of the putative GM structures of Zn clusters. Accord-ingly, we include a complete discussion of this issue in the next section.

### 3

### Results and Discussion

3.1 Putative Global Minimum Structures

The putative GM structures that emerge from our study are
shown in Figures 1-5. A tri-capped trigonal prism (TTP) is
obtained for Zn9. The structures in the size rangeN=10−14
are based on adding atoms to that TTP unit. In some cases,
such as Zn+_{11} or Zn+_{12}, the adatoms have an anomalously low
coordination which is not expected in clusters of a metallic
element. This feature, which recurrently appears for some of
the bigger size clusters, has been analysed in a recent report,41
where we have shown that those adatoms introduce localized
insulating features in an otherwise metallic-like electron
den-sity distribution. Therefore, these clusters feature an
unprece-dented coexistence of two different electronic phases (metallic
and insulating) within a single nanoparticle.

### Zn

_{17}+

### (C

_{2v}

### )

_{Zn}

17

### (D

5h### )

### Zn

17 −### (C

### Zn

_{18}+

### (D

_{5h}

### )

### Zn

_{18}

### (C

_{2v}

### )

_{Zn}

19

### (C

2v### )

### Zn

19 −### (C

_{3}

### )

### Zn

_{20}

### (C

_{3}

### )

### Zn

_{20}−

### (C

_{3}

### )

### Zn

_{21}

### (C

_{1}

### )

_{Zn}

21
−
### (C

_{1}

### )

### Zn

_{23}

### (C

_{1}

### )

### Zn

24### (C

s### )

### Zn

26 +### (C

_{1}

### )

s### )

Fig. 2Putative GM structures and approximate point group symmetries of selected zinc clusters withN=17−26 atoms. Yellow color is used to distinguish the interior or core atoms. Rest of the caption as in Figure 1.

and neutral/anion clusters is just due to a different choice of the three common atoms. In fact, the low energy excitations (isomers) identified for Zn15are just different ways of joining two TTP units, implying that the energy cost of reorienting those two units is much less than the energy needed to destroy one of them. This might lead to interesting thermal behavior at low temperatures, with fluxionality provided by the relative motion of otherwise “rigid” TTP units. The GM structures for sizeN=16 are essentially obtained by adding one atom to the 15-mer. In the small size rangeN=9−16, all the atoms still belong to the cluster surface. This is already an indication that zinc clusters are less compactly packed as compared to clus-ters of other typical metals such as sodium42, aluminum43–45, or silver46, as all those clusters have already developed at least one interior or core atom in this size range. We also notice that the GM structures of neutral, cation and anion are different at many sizes, a feature which will also persist in the bigger clus-ters discussed below.

N=17 is the critical size for the stability of structures
with-out core atoms. Both the cation and the neutral adopt a hollow
cage structure, obtained by capping the five square faces of
a hollow 12-atom decahedron, and retains full D_{5}_{h}
symme-try in the neutral state. The cation undergoes a slight
Jahn-Teller distortion that lowers the symmetry to C2v. The cage

is nearly spherical in shape although it shows a slight prolate distortion, i.e. it is more elongated along its 5-fold symmetry axis than along its equatorial plane. Notice that a “standard” capped decahedron would instead have a significantly oblate shape as the five capping atoms would be more distant from the cage center. However, upon relaxation of that initial struc-ture, the originally square faces of the decahedron elongate

along the direction of the 5-fold axis (becoming rectangular facets) while the capping atoms undergo an inwards relaxation and approach the cluster center, resulting in a nearly spherical cage. Hollow cages of a metallic element, that moreover are the GM on the potential energy surface, are very exotic and interesting species as they may be used as hosts for a variety of dopants. In the case of zinc, they are particulary interesting as metallic zinc is widely used in corrosion protecting lay-ers.47 Therefore, zinc nanocoatings may be useful to protect the potentially interesting properties of the embedded mate-rial from the environment and other external influences. In a recent report,48 we have shown that Cr@Zn17 is a magnetic superatom with the chromium atom placed in the cage cen-ter. This cluster preserves the whole magnetic moment of the isolated chromium atom (6µB), even after coalescence of two

such units or after exposure to an oxygen atmosphere. The
GM structure of Zn−_{17}is still based on the capped decahedron,
but already contains a pseudointernal atom that occupies the
center of the decahedron.

In the size rangeN=18−26 the GM structures contain a single core atom. The 18-mer is obtained by filling the cen-tral position of the Zn17cage. Full D5hsymmetry is preserved

only in Zn+_{18}, while the neutral and anionic clusters distort and
have only C2vsymmetry. An additional capping atom results

### Zn

_{28}+

### (C

_{2}

### )

### Zn

_{28}

### (C

_{2}

### )

### Zn

_{28}−

### (C

_{1}

### )

### Zn

_{28}2−

### (D

_{3}

### )

### Zn

_{29}

### (C

_{2v}

### )

### Zn

_{29}

### (C

_{2v}

### )

### Zn

29### (T)

### Zn

_{30}

### (C

_{3}

### )

### Zn

_{30}−

### (C

_{s}

### )

### Zn

_{31}+

### (C

_{2}

### )

### Zn

_{31}

### (C

_{2v}

### )

### Zn

_{32}+

### (C

_{s}

### )

### Zn

_{32}

### (D

_{3h}

### )

### Zn

_{32}−

### (C

_{2}

### )

Fig. 3Putative GM structures and approximate point group symmetries of selected zinc clusters withN=28−32 atoms. Rest of the caption as in Figures 1,2.

amorphous GM structure.

With few exceptions, clusters withN=27−30 atoms
con-tain an internal dimer. ForN=27−28 the structures have
a prolate shape and little symmetry. Zn29 in its neutral state
has three nearly degenerate GM structures. One of them is
exceptional because it contains a single core atom surrounded
by a shell with one of the highest chiral symmetries (T). Cores
with two atoms are clearly favored in this size range, and the
special stability of the tetrahedral structure is due only to its
spherical shape and an electron shell closing effect (Zn29
con-tains exactly 58 electrons, a magic number of electrons in a
spherical jellium picture49,50). The HOMO-LUMO gap of the
tetrahedral structure is 1.6 eV, as compared to 0.75 eV for the
structures with two core atoms. The near degeneracy is thus
the result of a strong competition between electronic and
geo-metric preferences. The average distance between two surface
atoms in the T-structure is 2.60 ˚A, while the average core-shell
distance is 3.4 ˚A. This is just an extreme example of another
quite general and defining property of all zinc cluster
struc-tures withN≥18, namely the presence of a low-density core,
surrounded by a distant, rounded and crowded shell. Because
the Zn2_{28}−di-anion also contains 58 electrons, we decided to
perform unbiased optimizations for its structure and found that
it contains also a single core atom (see Fig. 3) and a shell of
D3symmetry, resulting from the removal of one atom from
the shell of Zn29. It is interesting to notice that all other
struc-tures for Zn2_{28}−(containing two core atoms) are unstable as the
calculated electron affinities of Zn−_{28}are negative, and only the
D3isomer of Zn−28displays a positive electron affinity, which
renders Zn2_{28}−as the smallest stable zinc di-anion. Its
HOMO-LUMO gap is 1.2 eV.

The two remaining degenerate structures of Zn29 are quite similar to each other. Both contain a decahedral shell with ap-proximate D5hsymmetry that encapsulates a zinc dimer, and

differ just in the orientation of that dimer with respect to the
cage frame. For Zn+_{29}and Zn−_{29}, these two structures continue
to be nearly degenerate global minima, but the T-isomer is
now much less stable. The stability of the T-structure thus
de-pends quite critically on the number of electrons. The GM
of Zn30and Zn+30is obtained by adding one atom to the core
of Zn29(T), which lowers the point group symmetry down to
C3. This is the second example we find in which the
clus-ter grows by adding atoms to the core rather than to the shell.
Zn−_{30} already contains three core atoms, although this
struc-ture is nearly degenerate with another one obtained by adding
a low-coordinated adatom to the C2vstructure of Zn29.

The core region of clusters with N=31−33 atoms con-tains three atoms in a triangular arrangement, which equips these clusters with an oblate global shape. The way in which the shell grows around this core is highly dependent on the charge state of the cluster and the number of atoms. Zn31, for instance, displays a mixture of hexagonal-closed-packed (hcp) and decahedral growth patterns. Zn32 is a perfect hcp crystalline fragment that retains full D3hsymmetry and so it

is the smallest cluster that has the same packing as bulk zinc.
In Zn+_{32}, the growth of the shell is different on both sides of
the triangular core: while on the front side it follows a
com-pact packing pattern, on the back side it adopts a less comcom-pact
simple hexagonal packing.

The size rangeN=34−38 features clusters with a
tetra-hedral 4-atom core. In Zn−_{34}, the shell preserves the full Td

### Zn

_{33}+

### (C

_{2v}

### )

### Zn

_{33}

### (C

_{1}

### )

### Zn

_{33}−

### (C

_{1}

### )

### Zn

_{34}+

### (C

_{1}

### )

### Zn

_{36}−

### (C

_{s}

### )

### Zn

_{38}+

### (C

_{3v}

### )

### Zn

_{38}

### (C

_{1}

### )

### Zn

−_{38}

### (C

_{1}

### )

### Zn

_{39}

### (C

_{2v}

### )

### Zn

_{40}+

### (D

_{2}

### )

### Zn

_{40}

### (C

_{2v}

### )

### )

1### (C

36### Zn

### )

1### (C

36### Zn

+### )

d

### (T

### Zn

34

Fig. 4Putative GM structures and approximate point group symmetries of selected zinc clusters withN=33−40 atoms. The Tdstructure of

Zn34is shown from two different perspectives. Rest of the caption as in Figures 1,2.

four interpenetrating TTP units (the four atoms of the
inter-nal tetrahedron being common to the four TTP units). The
corresponding neutral cluster adopts the same structure but
with a slight distortion that lowers the symmetry down to C2.
The HOMO-LUMO gap of Zn34is only about 0.5 eV, but we
observed a large gap between the LUMO and LUMO+1
lev-els, which motivated us to optimize the Zn2_{34}−di-anion. It
re-tains the full Tdsymmetry of the singly-charged anion, and its

HOMO-LUMO gap is 1.25 eV, implying that Zn2_{34}−is a doubly
magic cluster, having closed geometric and electronic shells.
Zn+_{38} also displays a highly symmetric (C3v) shell

surround-ing the tetrahedron, but the rest of GM structures in this size range are of low-symmetry and based on adding atoms to the Td structure of Zn−34. In particular, for Zn35we obtain a low symmetry structure with a large HOMO-LUMO gap of 1.2 eV, so the electron shell closing for 70 electrons persists even if the geometric shell closing doesn’t.

A structural transition in the core region occurs at size
N=39 and also for Zn+_{40}. Here the core continues to have four
atoms, but it is now planar and with a rhombus shape. This
transition towards a less compact core allows to pack a larger
number of atoms into a single shell of monatomic thickness
without modifying the number of core atoms, and it is
some-times observed in zinc clusters as a prelude to the change in
the number of core atoms. For both sizes, the shell preserves
many of the symmetries of the rhombus core.

Clusters with five core atoms are found for most sizes in
the intervalN=40−44. Zn40has a multiply twinned layered
structure with a trigonal bipyramidal core. Apart from some
relaxation of the outermost atoms, this structure can be cut out
from a perfect 54-atom decahedron. Zn+_{43} has the same core
and a shell that preserves all but the mirror plane symmetries
of the core, resulting in a chiral cluster with D3 symmetry.
Once more, we observed that a transition towards a less

com-pact 5-atom core, in this case a square based pyramid, occurs
for example in Zn−_{43} and Zn+_{44}. Neutral Zn43 and also Zn41
(not shown explicitly) are exceptional in this size range as they
feature the reentrance of 4-atom cores. In Zn43, the core is a
nearly flat rhombus and the structure contains a hollow site,
similar to that observed in Zn17.

Six-atom cores occur in clusters withN=45−48 atoms.
Here the reference structure is Zn46, a cluster with 92 valence
electrons and so an electronic shell closing according to a
spherical jellium model. This cluster is almost perfectly
spher-ical indeed. Its core is octahedral, and the rounded shell
main-tains a high chiral symmetry (D4) for the whole cluster. Its
large HOMO-LUMO gap (1 eV) and its compact shell without
defects allows to qualify this cluster as a doubly magic size.
All the structures forN=45,47,48 are based on removing or
adding atoms to this reference structure. In some cases such as
Zn+_{48}, we observe again low-coordinated, dangling, adatoms.

Clusters with N=49−53 atoms possess mainly 7-atom octahedral cores of C3v symmetry, obtained by capping one

face of the octahedron, which equips these clusters with an elongated (prolate) shape. Zn49 can still be viewed as grown from Zn46 via addition of three adatoms, but the remaining clusters in this size range do not longer show a resemblance to Zn46. Most of the structures have no symmetries (C1point group) despite there is a clear octahedral order in the core. The only exception is Zn52, for which the shell fully preserves the C3v symmetry of the core. This structure shows an

interest-ing packinterest-ing pattern: while the core is octahedral, the 45-atom
shell is icosahedral, in fact it is the same 42-atom shell that
occurs in a 55-atom icosahedron, with three atoms added on
one facet. Mixed packing patterns like this have been found in
several metallic nanoalloys,51_{but they are not usual in }
homo-geneous metallic clusters.

43

### (D

3### )

### Zn

+### Zn

43### (C

2v### )

−

43

### (C

s### )

### Zn

+44

### (C

2v### )

### Zn

46### (D

4### )

### Zn

+47

### (C

4### )

### Zn

+_{48}

### (C

_{4}

### )

### Zn

49### (C

1### )

### Zn

_{51}

### (C

_{1}

### )

### Zn

52### (C

3v### )

### )

### (C

_{Zn}

_{)}

### Zn

56### Zn (C )

### Zn (C )

### Zn (C )

### Zn

_{65}

### (C

_{2}

### )

### Zn

+66### (C

2### )

### Zn

−_{67}

### (D

_{3}

### )

_{Zn}

70### (D

3### )

### Zn

_{71}

### (C

_{2h}

### )

### Zn

73### (C

1### )

54### (D

2d 55 s### )

_{ (C}

2v

### Zn

### Zn

### Zn

### Zn

### Zn

### Zn

### Zn

55

− +

_{ (D}

3d

### )

### Zn

56### (D

2d### )

2 59 58 s

1 57 +

Fig. 5Putative GM structures and approximate point group symmetries of selected zinc clusters withN=41−73 atoms. Blue and green

colors are used to highlight two different surface facets in Zn70. Rest of the caption as in Figs. 1,2.

namely a tetra-capped tetrahedron, surrounded by a complete shell of D2d symmetry. The high symmetry and the absence

of vacancies or adatoms at the shell qualifies this cluster as a
geometric shell closing. The GM structures of Zn53and Zn−53
(not explicitly shown) are obtained by creating a vacancy on
the shell of Zn54, while the 55-atom clusters have one adatom
on top of the Zn54structure. For the Zn−_{55}anion, the adatom is
located at a higher symmetry site resulting in C2vglobal

sym-metry and a core with 9 atoms. Zn+_{56} still has an elongated
core, namely an octahedron with two atoms capping
diametri-cally opposed facets. This structure has a high D3dsymmetry

that is respected by the shell. Neutral and anion clusters with 56 atoms have instead a 10-atom tetrahedral core surrounded by a shell with D2dsymmetry. Zn+57contains one adatom on top of the 56-atom D2dstructure. Different core structures are

competitive in this size range, which results in a substantial structural diversity.

In the size range N=58−66, we observe a substantial
increase in the rate at which the core size grows. Sizes
N=58−60 have 9-atom cores. For Zn58the core is
octahe-dral, while forN=59,60 the core is a pentagonal bipyramid
with two capping atoms. This core can be viewed as a
frag-ment of a 13-atom icosahedron. SizesN=61−63 have no
rotational symmetries but contain a 10-atom icosahedral
frag-ment in their cores. For sizesN=64,65 the core is an 11-atom
icosahedral fragment. Clusters with 66 atoms and also Zn+_{67}

and Zn67 have 12-atom cores. All of them are icosahedral
except for Zn+_{66}, for which the core is an hcp fragment with
stacking sequence 3-6-3. The structures in the core thus seem
to be developing a well defined tendency towards icosahedral
packing, which is not seen in the free zinc clusters with 9-12
atoms. This is suggestive of important differences in the
phys-ical behavior and chemphys-ical bonding of zinc atoms in “bulk”
(interior) and surface regions.

72,73 already contain 14-atom cores and their structures are quite amorphous.

The two different exchange-correlation functionals
em-ployed (PBE and KBM) predict the same GM structures for
nearly all sizes, implying that PBE is a sufficiently accurate
approximation for most purposes. Only for a few sizes did the
KBM and PBE calculations result in different GM structures.
In those cases, however, it is only the EDOS of the KBM
struc-ture that matches the experimentally measured photoemission
spectra (see next subsection), so vdW dispersion effects,
al-beit small, are important for a quantitative comparison to
ex-perimental results. We observed that the few discrepancies
al-ways occur close to critical sizes at which the number of core
atoms increases by one unit. As an example, the PBE
predic-tion for Zn−_{17}continues to be a hollow cage, while the KBM
structure already contains one core atom. Another example
is Zn−_{30}, where PBE predicts a structure with two core atoms
and KBM a different one with three core atoms (in figures 1-5,
we have always quoted the more correct KBM structure when
it differs from the PBE prediction). In summary, the KBM
functional favors more compact geometries, and so it slightly
shifts down the critical sizes for the transition between
differ-ent core sizes: the first internal atom occurs in Zn+_{18}with PBE,
but in Zn−_{17}with KBM; The first cluster with three core atoms
is Zn+_{31}in PBE, but Zn−_{30}in KBM calculations, etc. The most
important observation is that the effect is systematic. This is
exactly the same trend previously identified in a study of
ce-sium clusters.52

We close this subsection with a brief comparison to the re-sults obtained in previous theoretical works on small zinc clus-ters. Michaelianet al.32reported global optimizations for zinc clusters of selected sizes employing a Gupta potential with pa-rameters fitted to bulk properties. The structures were later re-optimized at the DFT level of theory, and the putative GM were found to be disordered or amorphous structures. Ac-cording to our explicit calculations, the structures reported by Michaelianet al. are less stable than the ones reported here by as much as 1-2 eV. As explained in the previous section, the reason is that the bulk-fitted Gupta potential for zinc is not transferable to the nanoscale and thus is not representa-tive of the atomic interactions in real zinc clusters. The newly parametrized Gupta potential obtained in this work provides a much better agreement with theab initioresults, and predicts high-symmetry structures for nearly all sizes. Thus, our re-sults oppose previous claims about an expectedly amorphous structure of zinc clusters. Later on, Doye reported a dedi-cated and systematic basin hopping study of zinc clusters with N≤125 atoms, based also on a Gupta potential, and found a strong structural tendency towards distorted oblate Marks decahedra.53Although our DFT study confirms the existence of distorted decahedral packing for some sizes, most of the GM structures do not coincide with those reported by Doye.

The main qualitative feature of the DFT results, which is al-ready reproduced in Doye’s work, is the emergence of low-density cores surrounded by relatively distant crowded shells. This trend is however quantitatively enhanced by the newly parametrized potential and DFT results.

Wang et al.54 reported DFT-GGA optimizations for neu-tral zinc clusters with N=2−20 atoms. Their structures were employed also in later calculations of electronic prop-erties of zinc clusters.56,57Our results forN=9−15 are in full agreement with the structures shown in that paper. We locate more stable structures, however, for some clusters with N=17−20 atoms: For Zn17Wang predicts an atom-centered structure with D4dsymmetry that is more than 0.4 eV less

sta-ble than the hollow D5h cage according to our calculations;

for Zn20their putative GM structure is 0.2 eV less stable than
the C3structure located here. Liet al.55 also considered the
size rangeN=2−20 at the GGA level, although they do not
provide coordinate files nor point-group symmetries, so a
di-rect comparison by simple visual inspection becomes
compli-cate beyond 17 atoms. We identify a clear discrepancy at size
N=17, where an atom-centered structure is proposed as GM.
That structure is 0.2 eV less stable than the hollow cage in our
calculations. Gutsevet al58have recently reported all-electron
DFT-GGA results for sizesN=12,13, including both neutral
and singly-charged states. We obtain a good agreement with
their structural results except for Zn+_{12}. These authors do not
explain how they choose the trial structures to be optimized, so
we can just speculate that the possibility of singly-coordinated
or dangling adatoms (which we predict to occur for Zn+_{12})
per-haps was not explicity tried in their work as this is addmitedly
a weird feature. In any case, their putative GM structure for
Zn+_{12} is one of the excited isomers according to our
calcula-tions. Finally, Jellinek and Acioli reported DFT-GGA results
for neutral and negatively-charged magnesium clusters with
N=2−22 atoms. Magnesium and zinc are isovalent if we
do not include the deep and localizedd−band of zinc in the
electron count. Most of the GM structures that we find for
zinc clusters indeed coincide with those of Mg clusters, the
exceptions being sizes N=16,17,19 for the neutral series,
andN=16−19 in the anion series.

3.2 Electronic Properties

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### Intensity (Arb. units)

### Binding Energy (eV)

### 9

### 10

### 11

### 12

### 13

### 14

### 15

### 16

### 17

### 18

### 19

### 20

### 21

### 22

### 23

### 24

### 25

### 26

### 27

### 28

### 29

### 30

### 31

### 32

### 33

### 34

### 35

### 36

### 37

### 38

### 39

### 40

Fig. 6Comparison between experimental photoemission spectra (black lines) and theoretical electronic density of states (green lines) for zinc

essentially perfect. There are some other sizes (for example,
N=38), where the agreement is far from perfect but still fair.
At this size, we identified two nearly degenerate GM
candi-date structures, and a superposition of both EDOS reasonably
reproduces the experimental peak energies. Finally, there are
a few sizes (Zn−_{36}, Zn−_{49}, for instance) for which neither the
GM structure nor any of the metastable isomers identified in
the calculations can reproduce the experimental spectrum. We
conclude that the correct GM structure has not been found yet
for these sizes.

As a general rule, most sizes for which the agreement is not
perfect coincide with clusters for which theory predicts a
low-symmetry GM structure, usually accompanied by competing
structures which are nearly degenerate in energy. But for all
cases with a highly symmetric GM structure, well separated
in energy from all other isomers, the agreement with
exper-iment is very good. For example, the two-peak spectrum of
Zn−_{34}, or the highly structured spectrum of Zn−_{54}, can only be
matched by the corresponding geometric shell closings with
Tdand D2dsymmetry, which should be difficult to locate due

to entropic factors, and even more difficult to guess using in-tuition and hand-made initial structures. The agreement is es-sentially perfect also for the biggest clusters considered, with more than 60 atoms, which would not be amenable to a di-rect first-principles optimization. These observations imply that our unbiased search strategy worked quite well indeed, and that the combined EP-DFT approach is really necessary to unravel the structures of zinc clusters.

In a recent report,41 _{we have analysed in depth the }
elec-tronic shell structure of Zn clusters through the density of
states and its projections onto atomic orbitals; and the
elec-tronic density in real space through the analysis of two scalar
fields: the electron localization function (ELF)59and the
de-formation density (defined as the difference between the
self-consistent and the promolecular densities). Summarizing the
main findings of that work may be worthwhile here. Our
anal-ysis demonstrated that clusters without adatoms match quite
well the qualitative predictions of deformable jellium
mod-els. Accordingly, we locate the main electronic shell
clos-ings for clusters withNe=20,34,40,58,70,92,138· · ·

elec-trons, and for those sizes the cluster shape is close to perfectly spherical. In between the spherical shell closings, the cluster shape deformations are also in good overall agreement with jellium predictions at least for the smaller sizes, i.e. the dis-tortions are prolate-like right after an electron shell closing, pass through triaxial and become oblate as the new electronic shell is progressively filled. Notwithstanding these facts, the anomalously long separation between core and shell identified in zinc clusters (see previous section) reflects itself as a deep minimum along the radial direction in both the ELF and the deformation density, i.e. the relatively hollow space left be-tween core and shell is significantly depleted from electrons.

In fact, the minimum in the ELF is as deep as that found be-tween two units of a typical insulating material,41and this is clearly not a usual jellium feature. In fact, the detailed ELF analysis showed that Zn clusters can be viewed as consist-ing of two nearly independent metals: a three-dimensional and isotropic metallic phase located at the core, and a two-dimensional directional metal located at the spherical shell, which is stabilized by a connected network of three-center bonds reminiscent of an sp2−hybridization scheme. There-fore, even if the jellium picture remains valid to first order be-cause of the angular delocalization, the electron density along the radial direction shows some non typically metallic fea-tures.

Clusters with adatoms, which are observed for sizes follow-ing a spherical shell closfollow-ing, depart from jellium model pre-dictions due to one additional reason: the two valence elec-trons contributed by the adatom do not populate the LUMO of the parent cluster as expected from a metallic cluster. They rather take an “insulating” option, and contribute a newly formed statebelowthe bandgap, without significantly disturb-ing the EDOS of the metallic “host”. This is precisely the expected behavior when an atom is added to a separate band insulator. In such a case the filled orbitals of the atom would add to the fully occupied “valence band” level manifold, while its empty orbitals would become part of the unoccupied “con-duction band” levels. The ELF shows a very deep minimum in the region between the adatom and the rest of the cluster, indicative of a non-bonding interaction. These clusters are therefore best viewed as a “hetero-dimer” formed by an atom plus a metallic superatom, and the bond between atom and su-peratom is mainly of an ionic nature as demonstrated by an analysis of the charge transfers.41

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### 2

### 3

### 4

### Intensity (Arb. units)

### Binding Energy (eV)

### 41

### 42

### 43

### 44

### 45

### 46

### 47

### 48

### 49

### 50

### 52

### 53

### 54

### 55

### 56

### 57

### 58

### 59

### 60

### 61

### 62

### 63

### 64

### 65

### 66

### 67

### 68

### 69

### 70

### 71

### 72

### 73

Fig. 7Same as in previous figure, but for the size rangeN=41−73. Photoemission spectra were not measured for sizesN=63−67.

case, we show in figure 8 the EDOS of Zn_{69}, another
spher-ical electron shell closing with 138 electrons, but which is
more representative of generic zinc clusters. We have
pro-jected the total EDOS onto an angular momentum eigenbasis
centered on the cluster center of mass in order to reveal the
su-peratom labels. For this particular cluster, the energies of the
1Dand 2Ssuperatom shells overlap with the localized levels
coming from the semicored−orbitals of zinc, which causes
some fragmentation of those peaks. Apart from that, the
ex-pected jellium order is obtained up to the 1G shell, which
completes the 58-electron shell closing. After that closing,
the 1H, 2D, and 3S level manifold is filled to produce the
next electron shell closing at 92 electrons (the expected
addi-tional closing at 70 electrons is missed in this cluster). Notice
that, as expected from the discussion above, the 1H−levels are

on average more stable than 2D, which themselves are more stable than 3S. Similarly, the 1I−orbitals are most stable in the next manifold of levels which produces the 138-electron shell closing. The main conclusion from this analysis is that, although some stabilization of high angular momentum lev-els is indeed observed, the effect is not intense enough as to open new gaps in the EDOS. This observation is relevant concerning a phenomenological level interchange model ad-vanced by Diederichet al.29 in an attempt to rationalize the magic numbers observed in mass spectra of magnesium and other divalent clusters. For example, they proposed that the observed magic character of Mg40 might be explained by a large stabilization of the 1Hshell as compared to 2Dand 3S shells (which would open a gap at Ne=80 electrons), and

accu--12 -10 -8 -6

Binding Energy (eV)

100 200 EDOS (electrons/eV) d S P D F G H I

1S21P6[1D102S2]1F142P61G18[1H222D103S2][1I263P62F14]

Fig. 8Electronic density of states of Zn69, projected onto a spherical harmonics basis centered on the cluster center of mass.

The black line shows the contribution of the semicored−electrons

of zinc, which goes out of scale in this plot. The assignment of levels with angular momentum superatom labels is shown at the top of the plot.

mulation of positive jellium background density close to the cluster surface. The results shown in Figure 8 confirm that an interchange of levels certainly does not occur in zinc clusters, which already display an anomalously high concentration of positive ionic density at their surface, so we believe it is im-probable that anything close to a true level interchange occurs in magnesium clusters. In fact, most of the identified magic numbers are the same for Mg and Zn clusters. In the next subsection, we will show that the additional magic numbers of zinc clusters (those not easily explained by electronic shell closings) can be ascribed to geometric shell closing effects.

In the upper part of figure 9 we display adiabatic electronic properties of ZnN clusters: ionization energies (IP), defined

as [E(Zn+_{N})−E(ZnN)], are shown on the left side; electron

affinities (EA), defined as[E(ZnN)−E(Zn−N)], are shown on

the right side. Being adiabatic quantities, they include also a contribution from the structural relaxation that occurs after the detachment/attachment of one electron. Notice, for example, that the EA values are not the same as the vertical detachment energies of anions, which can be read off directly from the DOS/PES plots.

As it is well known, the electronic properties of small metal clusters usually display strong fluctuations as a function of size. Neutral clusters with a specially stable electronic shell structure are expected to show an enhanced stability against dissociation and therefore to be in close correspon-dence with the magic numbers that will be analysed in

5.25 5.5 5.75 6 6.25 6.5 IP (eV) 1.5 2 2.5 3 3.5 EA (eV)

10 20 30 40 50 60 70

N

3 4 5

Fund. Gap (eV)

10 20 30 40 50 60 70

N
3.8
4
4.2
4.4
4.6
χ
(eV)
15
1720
2529_{3235}

37 9 10 10 17 20 37 28 32 35 9 19 27 30 31 34 33 36 10-11 1720 41 32 35 29 10-11 1720-21 29 33 36 9 15 18 27 31 34 46 49 69 71 41 47 57 56 72 40 45 46 68 69 46 69 40 45 43 68 72 56 54 56

Fig. 9Adiabatic ionization energies (upper left), adiabatic electron affinities (upper right), fundamental band gap energies (lower left)

and electronegativities (lower right) of ZnNclusters. The most

relevant sizes in the discussion, associated with sharp changes in these electronic indicators, are explicitly annotated in red colour.

Zinc being divalent, each atom contributes two electrons to
the total valence electron count and so only neutral clusters
have an even number of electrons. On the other hand, all the
zinc clusters considered in this study adopt an electron
con-figuration with the minimum possible spin multiplicity, i.e. a
singlet for neutrals and a doublet for both cations and anions.
With these considerations in mind, we may provide some
in-terpretation of the EA maxima and IP minima. Marked
lo-cal maxima in the adiabatic EA curve identify clusters which
would like to gain one electron, so they are expected to be
very stable as anions as those anions would be just one
elec-tron short of an elecelec-tronic shell closing. Maxima in the EA are
obtained forN=9,19,27,31,34,40,45,54 and 68, all of them
correlating indeed with specially stable anion sizes (see next
subsection). Notice that local maxima in the IP correspond to
Zn+_{N} cations which are also short of one electron to close the
shell. Accordingly, we observe that many of the neutral magic
numbers are preserved in the cations. Marked local minima in
the IP curve, on the other hand, identify clusters with a loosely
bound HOMO populated with two electrons, and removing
one electron would leave the cation with a single electron in a
loosely bound HOMO (one excess electron as compared to a
closed shell). These cluster sizes might therefore be expected
to preserve some electronic stability as cations as well. The
local IP minima atN=30,33,36,47,52−53 and 72 indeed
coincide with relatively stable cluster cations, although not
al-ways with a local stability maximum (see next subsection). In
summary, our calculations demonstrate that, as compared to a
genuine shell closing which can only occur in neutral clusters,
charged clusters with one electron less are more stable than
clusters with one electron in excess.

In the lower part of figure 9 we provide vertical electronic properties, which include no geometry change and are thus not expected to correlate so perfectly with the size dependence of the absolute stabities. The left graph shows the fundamental gap, defined as (VIP-VEA). One half of that would be just the definition of chemical hardness. The right graph shows the electronegativity (or the negative of the electronic chemical potential) defined as (VIP+VEA)/2. These two quantities are of fundamental importance in reactivity studies, as the elec-tronic processes that occur in typical reactions are simply too fast as compared to vibrational frequencies.

The fundamental gap shows the expected average trend to decrease as the cluster size increases, associated with the grad-ual development of a metallic and more reactive phase. It re-produces the substantial gap closure atN=18−19 identified in the experiments as well as the re-opening atN=20. The strong size oscillations observed for sizes N <46 correlate quite well with those in the adiabatic IP curve. A curious fea-ture is that Zn11 with 22 electrons has a wider gap than Zn10 which is a closed shell cluster with 20 electrons. As discussed in our previous paper,41this anomaly is due to coexistence of

metallic and insulating features in Zn11. The adatom in this cluster contributes a localized insulating level below the band gap rather than occupying the LUMO of Zn10, and so Zn11 continues to have a closed electronic shell. A similar effect occurs forN=21 and 47, which also maintain a wide gap af-ter a jellium shell closing. According to the experiments of Issendorff and Cheshnovski27,28, the closing of the gap with increasing size should become smoother for sizes larger than about 40, apart from recurrent re-openings associated to elec-tron shell closings. The theoretical results are in agreement with this prediction, including the re-opening of the gap ob-served for Zn56and Zn69.

The more electronegative clusters, which would be the more oxidizing agents in a reaction involving Zn clusters, occur at sizes which are in good correspondence with the local max-ima in the EA curve, at least for clusters with more than about 20 atoms. Therefore, we conclude that electronegativity max-ima are mainly dominated by the electron affinity contribution in that size range. For N<20, however, the electronegativ-ity maxima are rather a consequence of a large ionization po-tential. Similarly, the less electronegative clusters are the re-sult of very low ionization potentials forN>20, but correlate with low electron affinities forN<20. Once more we find that clusters with adatoms (Zn11and Zn21, for example) have unexpected vertical electronic properties, as their electroneg-ativities are even lower than those of the nearest closed shell clusters (Zn10and Zn20, respectively).

3.3 Cluster Stabilities

Figure 10 shows two different stability measures: the cohesive
energy (or binding energy per atom)Ecoh(N) =E1−E_{N}N and
the second energy difference ∆2(N) =EN−1+EN+1−2EN.

The cohesive energy quantifies the total internal energy con-tent of a cluster and is therefore a measure of its global (or absolute) stability. ∆2provides a more “local” stability mea-sure, by comparing the energy of a cluster of size N to that of clusters with neighboring sizes, and so it is a more suit-able quantity to interpret the results of abundance mass spectra measured on an evaporative ensemble of clusters. The cohe-sive energies show an oscillating pattern about the average be-havior (itself obtained by a smooth fit to the numerical data). Neutral clusters withN=10,17,20,29,32,35,46,54,65,and 69−71 have an enhanced stability as compared to that av-erage. The cohesive energies of charged clusters can be anal-ysed in a similar way. Overall the oscillations are in qualitative agreement with the enhanced electronic stabilities predicted in the previous subsection. It demonstrates that the electron shell structure is the most important factor determining the abso-lute stability of ZnNclusters in this size range, with geometric

symmet-ric and compact structures with a perfectly icosahedral core). The only exception to this rule is Zn54which is a geometric shell closing with an open electronic shell, and which is more stable than the electronic shell closure that occurs at Zn56. One reason for this strange behavior is that Zn56contains 10 core atoms, which is more than optimal for that size. In fact, 10-atom cores are not recovered until N=61, so it seems that Zn56achieves an electronic shell closure at the cost of an un-favourable atomic shell structure.

-0,06 -0,03 0 0,03 0,06 Ecoh -E ave (eV) -0,5 0 0,5 ∆2 (eV) -0,5 0 0,5 1 1,5 ∆2 (eV)

10 20 30 40 50 60 70

N -1 -0,5 0 0,5 ∆2 (eV)

10 _{17 20}

15 26
28 30
3235,36
25
41
27
46,47 54
54
59_{62}
65
69

3134 _{45}

10 _{15}17
20
25 29
3235
37 41
46
56

59 6265 69 71

15 19 27 29 31 34 40 46

56 59 62 65 68 71 10

20

28 30 35,36 46,47

6569-71

10 17

20

29 32 35 46

69-71 65

9

15

19 _{29 31 34} 46

68-71 39 45 72 54 54 56 54 56 54

Fig. 10Two different stability measures for Zn clusters. The upper

graph shows the PBE cohesive energies, referenced toEave, which is

a four-parameter fit of the form

Eave=A0+A1N1/3+A2N2/3+A3N. The three lower graphs show

the PBE second-energy differences. Clusters with enhanced stability (or magic sizes) are shown for each of the stability indicators. Black, red and green curves refer to cations, neutrals, and anions, respectively. KBM results are shown for cations in a restricted size range with the dashed black curve, which has been vertically shifted to help visualization.

To make connection with experimental abundance spec-tra, we turn now to an analysis of the second energy dif-ferences. First, we compare our results for cations with the mass spectra reported by Diederich et al.29. Marked

abun-dance minima are observed in the experimental mass
spec-tra at N=12−14,22−24,29,31,34,37−39,45,53. All of
them are well reflected in our theoretical results either as
sub-stantial drops in the cohesive energies or negative values of
the second energy difference. The experimentally measured
abundance maxima are N =10,(15),20,26,28,30,32,35−
36,41−42,46−47,54,59,62,65,69,72. The agreement with
our theoretical predictions is essentially perfect, suggesting
that the identified GM structures are realistic also for cations.
A small discrepancy between experiment and PBE results is
the maximum predicted by PBE for Zn+_{17}, which is absent from
the abundance spectrum. To address this issue, we performed
systematic KBM calculations (shown with a dashed line) in
the restricted size rangeN=9−21, due to their significantly
higher computational expense. Remembering that the KBM
and PBE GM structures of Zn−_{17}were found to differ (see
pre-vious subsection), it is not unexpected to observe some
dif-ferences between PBE and KBM stabilities. In the case of
cations, we find that the KBM and PBE GM structures
coin-cide in this size range, yet the vdW correction to the stabilities
is slightly size-dependent, and Zn+_{17}becomes destabilized
rel-ative to Zn+_{16} and Zn+_{18}. The stability maximum at N=17
dissappears in the KBM results thus improving the agreement
with experiment.

As compared to the cohesive energies, the second energy
differences identify additional magic sizes, that indeed
cor-relate with enhanced experimental abundances for cations.
We notice that most of those additional sizes (for
exam-ple,N=15,41,59,62,65) are located within size intervals of
lower-than-average absolute stability, so its abundance in the
spectra is only due to their higher local stability, which may
have an electronic (N=15,41, see figure 9) or a geometric
(N=59,62) origin. We also notice the emergence of
appar-ent “magic number pairs”, which are also a peculiar feature of
the experimental mass spectra. These occur for cation sizes
bracketing an electron shell closing (which can only occur
in neutral clusters). For cations, “magic pairs” are observed
for N =10−11, 20−21, 32−33, 35−36, and 46−47,
as for all those sizes the ∆2 value is large and positive. In
some cases, the bigger cluster in the pair contains a
singly-coordinated adatom with insulating-like features. But in all
cases, theory and experiment agree in identifying the smaller
cluster as more stable within each pair. In particular, Zn+_{36}and
Zn+_{47} stand out as the most stable cations with one unpaired
electron outside a closed electronic shell.

stabili-112 Chapter 5. Clusters of divalent metals

5 10 15 20 25 30 35 40 45 50

55 60 65 70 75 80 85 90 95 100 105 110 115 120

120 125 130 135 140 145 150 155 160 165 170 175 180 185 190 195 200 31 25 46 34 27 19 9 3 x10 116 54 68 135 x55 x400 155 139 In te ns ity

Cluster size, *N*

Figure 5.9: Mass spectrum of zinc cluster anions.

with di↵erent laser energies (h⌫= 6.4 eV and 4.02 eV) are presented in the appendixH. The spectra in Fig.5.10are cut at a binding energy of 5 eV due to the appearance of two-photon e↵ects (photoelectron spectra of the neutral zinc clusters) at higher BEs for all but the smallest sizes. In most of the spectra one can observe a single peak at low binding energy, which indicates the highest occupied single electron state in the cluster, and a group of peaks at higher binding energy, which represent electron states with more negative total energies. As in the case of magnesium [123] the uppermost peak is assumed to be the lowestp-band state, which is occupied by the single additional electron of the cluster anion, and all other peaks are assumed to bes-band states. The di↵erences between the two highest peaks in the spectra therefore represent the excitation band gaps of the corresponding neutral clusters (in the geometry of the anions) [99].

In Fig.5.10strongly structured spectra are observed, suggesting a series of highly degenerate levels (though not necessarily a free-electron shell structure). Most of the cluster sizes up toN= 34 exhibit some band gap at the threshold. This band gap decreases rapidly from sizeN= 3 to sizeN= 10; for larger sizes only a slow decrease is visible. Figure5.11shows the size dependence of the band gap. The existence of a significant gap at least up to sizeN= 25 (51 electrons) indicates that zinc clusters in this size range have not fully undergone the transition to a metal and therefore behave like semiconductors.

Fig. 11Abundance mass spectrum of cluster anions, Zn−_{N}.

ties predicted by theory. Magic pairs are now expected at
N=9−10,19−20,31−32,34−35,45−46,68−69, and
many of them are indeed observed both in theory and
experi-ment. In most cases we observe again that the smaller cluster
in the pair is clearly more stable, and moreover this assymetry
in the stabilities around a closed shell is more pronounced than
in cations. Zn−_{46} is the only exception to the general rule, as
it is more stable than Zn−_{45}. This points to a substantial
con-tribution of the geometric shell closing to the stability of that
particular cluster size, as it is the only magic number which
is the same in the cation, neutral, and anion stabilities. This
is a sensible result as Zn_{46} is a doubly magic cluster,
hav-ing simultaneously closed electronic and geometric shells. A
similar double-closure effect occurs for Zn29 and Zn32in the
neutral series and would be expected for Zn2_{34}−in the di-anion
series.

### 4

### Performance of the Gupta potential

A final interesting point in our discussion is that the gross
structural features of most clusters are already captured by
the Gupta potential. This is of course rewarding, but at
the same time is strange: as explained in our previous
re-port,41the chemical bonding at the shell of zinc clusters
dis-plays a substantial directionality which is reminiscent of an
sp2−hybridization mechanism, and the Gupta potential
cer-tainly does not include any anisotropic interactions, at least not
in an explicit way. It is possible, however, that the many-body
character of the interactions can produce some effective
direc-tionality effects. As shown in the theory section, the energy
expression depends exclusively on two independent
parame-ters when expressed in reduced units, and we conveniently
choose those parameters asλ =q/p and χ = _{ξ}Aexp_{exp}(_{(}p_{q}_{)}). We

would like to analyze the physical meaning of those param-eters in order to explain why is the Gupta potential able to predict these exotic structures for metallic clusters.

5 10 15

Reduced Distance -1 0 1 Reduced Energy λ=0.1 λ=0.2 λ=0.3 λ=0.4 λ=0.5

0 5 10 15

Reduced Distance χ=100 χ=50 χ=20 χ=10 χ=5 χ=1

0 5 10 15 20

Reduced Distance Na Cu Al Au Pb Zn(b) Zn(c) χ=100 λ=0.4

Fig. 12The left and middle graphs show, respectively, theλ−and

χ−dependences of the reduced Gupta energies of a perfectly square

tetramer as a function of the nearest-neighbor reduced distance. The

right graph shows similar plots for selected metals24,60_{. Zn(b) and}

Zn(c) refer to the bulk and cluster fitted potential for zinc, respectively.